A first principle study of pressure induced structural and electronic properties in neptunium bismuthide
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications63A First Principle Study of Pressure Induced Structural andElectronic Properties in Neptunium BismuthideJagdish Pataiyaa, b*Chandrabhan Makodeb, A. Singhc, Mahendra Aynyasd, Sankar P. Sanyalaa, cDepartment of Physics, Barkatullah University, Bhopal, 462026, Indiaa, bSagar Institute of Research and Technology, Bhopal, 462041, IndiadDepartment of Physics, C.S.A. Govt. P.G. College, Sehore 466001, IndiaE-mail of corresponding author: email@example.comAbstractWe have examined the pressure induced structural and electronic properties of neptunium monobismuthides.The total energy as a function of volume is obtained by means of self-consistent tight binding linear muffin-tin-orbital (TB-LMTO) method within the local density approximation (LDA). It is found that NpBi is stable inNaCl – type structure under ambient pressure. We predict a structural phase transition from NaCl-type (B1-phase)sructure to CsCl-type (B2-phase) structure for NpBi in the pressure range of 11 GPa. We also calculate the latticeparameter (a0), bulk modulus (B0), band structure and density of states. From energy band diagram it is observedthat NpBi exhibit metallic behaviour. The calculated equilibrium lattice parameters and bulk modulus are ingeneral good agreement with available experimental data.Keywords: Structural phase transition; Electronic band structure; Metallic.1. IntroductionThe actinide based compounds are endowed with several physical properties due to the presence of f –electrons.The f-electrons are generally less localised than in the corresponding lanthanides, which explains the itinerantbehaviour at the beginning of the series, but for elements beyond Pu the increased nuclear charge causes the forbitals to overlap less, and crossover from itinerant to localised f electron behaviour occurs [1-3]. Considerabletheoretical but few experimental studies on plutonium binary compounds have been reported during the last fewyears. Gensini et al.  have studied the high pressure behaviour of NpBi by using anvil cell and high pressureX-ray diffraction measurements and reported that NpBi exhibit first order crystallographic phase transition fromNaCl (B1) to CsCl (B2) structure at high pressure. It is well known that with increasing atomic number, the f-shells become smaller and thus are more localized implying a smaller band width . This localization is alsofavoured from lighter (e.g. P) to heavier anions (e.g. Bi). In this context, it will be interesting as well toinvestigate the structural phase transition in NpBi.In the present study we have investigated, for the first time, thehigh pressure structural and electronic properties of neptunium monobismuthides (NpBi) at ambient and highpressure using ab initio Tight Binding-LMTO with LDA. In the section 2, we briefly describe the method oftotal energy calculation which will be followed by results and discussion on structural and electronic propertiesin section 3.2. Method of CalculationThe total energy, structural stability, electronic band structure (BS) and density of states (DOS) of neptuniummonobismuthides is calculated by using tight binding LMTO (TB-LMTO) method  within local densityapproximation (LDA) . The Von – Barth and Hedin parameterization scheme  has been used for exchangecorrelation potential. NpBi crystallize in B1-type (NaCl) structure with Space group Fm-3m (no. 225) at ambientpressure. In B1 structure, Np atoms occupy at (0, 0, 0) and Bi atoms at (0.5, 0.5, 0.5) positions respectively. Thecalculations were performed for 8000 k- points (20x20x20 k3grids) in the Brillouin zone for both B1 and B2structures. The E and k convergence were checked subsequently. The total energies were calculated by changingthe volume from 1.1 to 0.70Vo, where Vo is the equilibrium cell volume at ambient pressure. The calculated totalenergies as a function of volume for NpBi in B1 and B2 structures were fitted to Birch equation of state to obtainpressure – volume (P-V) and pressure-enthalpy (P-H) relation, finally leading to equilibrium lattice constants (a0)and bulk modulus (B0).3. Result and discussion3.1. Structural propertiesThe structural stability of NpBi has been examined by calculating the total energy as a function of volume inambient (NaCl phase) and at the high pressure (CsCl phase) structures and the results are shown in Fig. 1. TheNpBi, as is seen from Fig.1. transform to CsCl structure on compression. The calculated value of equilibriumlattice constant in the NaCl Structure is 6.00Å for NpBi, which agree fairly well with the experimental andtheoretical data  shown in table 1. The structural phase transition is determined by calculating the Gibbs free
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications64energy (G) for two phases (B1 and B2), which is given by G=Etot + PV - TS. Since the theoretical calculations areperformed at T= 0K, Gibbs energy becomes equal to enthalpy (H) (H = Etot + PV). For a given pressure, a stablestructure is one for which enthalpy has lowest value and the transition pressure (Pt) is determined at which theenthalpies of two structures are the same. Following such a procedure, the phase transition pressures (Pt) forNpBi is calculated for a B1 – B2 transition. The phase transition pressures have been estimated as 11 GPa NpBi,with volume collapse of 7%. The pressure – volume relationship or equation of states for NpBi is shown in Fig.2.The insets show the variation enthalpy as a function of pressure for respective compounds. In the B2 phase thecorresponding lattice parameter is 3.60Å. In addition to the above structural properties, the values of bulkmodulus (B0), calculated by using Birch equation of state, which has been shown in Fig.1. (for energy as afunction of pressure). The calculated results are presented in Table 1 for NpBi .Table 1: Calculated ground state properties of NpBiSolid Lattice Constant(Ao) Bulk Modulus(GPa) PhaseTransition Pressure(GPa)SolidNpBi Pre.B1 B2 B1 B2 116.00 3.60 82 141 -----Exp. 6.438a ------------ -----aRef. 3.2 Electronic PropertiesAn exact understanding of the electronic structure of NpBi is an extremely challenging problem, because of theitinerant behaviour of their 5-f electrons. However a qualitative picture of their electronic properties can bedrawn by comparing these properties for NpBi.We have, therefore, calculated the electronic band structure (BS) and density of states (DOS) of this compoundin B1 and B2 phases and plotted them in Figs. 3(a-b). It is seen from Fig.3. that both this compound are metallicin nature in B1 phase at ambient pressure.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications65To understand the band structure of NpBi qualitatively in Figs. 5, we have plotted the partial density of states (P-DOS). Highly localised Np-f band stays above the Fermi level at ambient, and moves marginally towards Fermilevel on application of pressure.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications664. ConclusionThe structural phase transition due to high pressure and electronic properties of NpBi has been studied using theTB-LMTO method. This compound undergoes a structural phase transition to B2 structure at 11GPa and is foundto be metallic in both the phases.AcknowledgementsThe authors are thankful to Dr. V. Srivastava and Mr. Tejash M. Tank for useful discussions and CSIR, andUGC for financial assistance.ReferencesJ.M. Leger, Physica B 190 (19993) 84-91.S. Dabos-Seignon, U. Benedict, S. Heathman, J.-C. Spirlet, M. Pagès, J. Less Common Met. 160 (1990) 35–52.L. Petit. A. Savane, W. H. Temmerman, Z. Szotek, Euro. Phys. J. B 25 (2002) 139-146.M. Gensini, R. G. Haire, U Benedict, F. Hulliger, Physica B 190 (1993) 75.O. Vogt and K. Mattenberger, J. Alloys and Comp. 223 (1995) 226-236.O.K. Andersen, Phys. Rev. B 12 (1975) 3060–3083.O.K. Andersen, O. Jepsen, Phys. Rev. Lett. 53 (1984) 2571–2574.U. van Barth, L. Hedin, Phys. C 5 (1972) 1629–1642.Mersse y, Heathman S, Rijkeboer C, Rebizent J, J. Alloys and Comp. 284 (1999) 65- 69.O. Jepson, O.K. Andersen, Solid State Commun 9 (1971) 1763-1767.W. Kohn, L.J. Sham, Phys. Rev. A 140 (1965) 1133–1138.
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar